1 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 6 Kinam Kim and Dong Jin Jung Samsung Electronics, S. Korea 1. Introduction Silicon industries have notched up notable achievements of computer-related technology over the past two decades, leading to rapid progression in information technology (IT). As a result of such a great improvement in IT applications, it is now not unusual to find mobile applications such as personal digital assistants, mobile phones with digital cameras, smart phones, smart pads able to access the Internet and hand-held personal computers. These mobile applications currently require an array of single-functioned conventional memories as they are not sufficient individually in functionality, but must combine their separate functions. For example, dynamic random access memory (DRAM) is capable of processing massive amounts of data speedily (e.g., main memory in personal computers and servers). DRAM is highly scalable (several gigabit are commonly accessible), but requires lots of power consumption even in stand-by mode (~10-3 Ampere) because of the necessity of refreshing cycles in its operation. By contrast, static random access memory (SRAM) saves power 1 because its stand-by current is a few micro-amperes. The demerit of SRAM is not readily to make it high density. This is due to the fact that its unit memory element consists of four complementary metal-oxide-semiconductor (CMOS) transistors along with two conventional transistors. SRAM s cost-benefit ratio is too high because the 6 components need much more area per unit bit memory. Data retention of both DRAM and SRAM is volatile in bit-storing nature when power goes off. In contrast to these two memories, flash memory is non-volatile. However, operation voltage during either write or erase on flash memory is too high to use the raw voltage-level of power input, Vcc (the term of Vcc comes from collector to collector voltage in a bipolar transistor). Thus during the write or erase operation, internal dummy operation (so called charge pump ) are used to pump up the input power Vcc to 5 times more than Vcc level; this is crucial in flash memory devices due to imbalance of read and write energy. The reason why the memory needs to boost the write/erase voltage up to such a high level is that hot carriers, e.g., high energy electrons, are forced to be injected through tunnel oxide to a floating gate of the transistor structure. As a result, there are two kinds of performance restrictions for use of IT applications. Writing speed of flash memory is not fast enough of an order of several milliseconds. That 1This is not necessarily true because the stand-by current of SRAM begins to exceed DRAM s in a deep sub micron scale due to involvement of high field junction.
2 118 Ferroelectrics - Applications makes the erasing speed of the device to be in the range of tenths of seconds. Another drawback of the device is endurance, which is defined as cycle times to write data in a memory cell. Generally, while write endurance of DRAM and SRAM is more than cycle 2 (10 15 corresponds to equivalent 10 years for use), flash memory has approximately 10 6 cycles at most as writing endurance. In addition to flash memory, there is another non-volatile memory, so called electrically erasable and programmable read only memory (EEPROM). However, EEPROM has the same limitations in flash memory due to structural and operational similarity of the unit memory cell in flash memory. To compensate for the aforementioned disadvantages of conventional memory devices, mobile applications in the IT world have adopted a combination of individual memories, which give several penalties such as a large volume of space to pack them all and complex time adjustments to synchronize them as well. As needs of IT technology are pushing forward to many functional requirements including much faster Internet access and far more image processing, this combining approach has a limitation to apply them to those for mobile uses. Therefore, it is strongly desirable to develop an ultimate memory solution as a single memory platform, possessing positive features of the individual memories but excluding their disadvantages. The feature of the ideal memory should have fast operation for speedy communication, high density for massive data-processing, non-volatility and low power consumption for portable applications. Among many candidates of ideal memory devices, a memory device to use ferroelectric properties, so called ferroelectric random access memory (FRAM), was proposed and experimentally explored in terms of 512-bit memory density (Evans & Womack, 1988). This is because its functional feature is similar to that of an ideal memory. This is thanks to the bistable state of ferroelectrics at near ambient temperature. There are several important characteristics worth mentioning. First, since core circuitry for the memory does not require stand-by power during quiescent state and the information remains unchanged even with no power supplied, it is thus non-volatile. Second, configuration of unit memory element is similar to that either of flash or of DRAM, allowing it to potentially become cost-effective high density memory. Third, speed of ferroelectric memory could be very close to those of the conventional volatile memories such as DRAM and SRAM. This is, in practice, because repeating the polarization reversal-read and write operation, does not need boost up base voltage unlike flash memory, stemming from balance of read and write energy of the same order of magnitude (Kryder & Kim, 2009). A good example of this is that, according to literature published recently, one of the FRAMs as a non-volatile memory has attractive memory performance such as fast access time of 1.6 GB/sec, negligible stand-by current of less than 10 micro-ampere, and low voltage operation of less than 2.0 V even in read and write action without erase operation (Shiga et al., 2009; Jung et al., 2008). Since then, there have been tremendous improvements in FRAM developments, migrating from sub-micron to nano scale in technology node. As such, this chapter is categorized into two: First demonstrates 2Provided a clock frequency f of a microprocessor in an embedded system is 20 MHz (the fastest one in 2006 is about 5 MHz), reference counts necessary for cycle times per a year, is less than 1E13 in spite of considering 2% of strong data-locality in data memory. Note, the reference counts per a second is proportional to the products of frl, where f is a clock frequency, r is ratio of number of cycles in read and write operation to unit cycle and L is a constant of representing data-access locality. We will discuss this more in section 3.2.
3 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 119 reminiscent of how memory technologies penetrate technological barriers to match the Moore s law. Also, authors are here trying to give an insight of how silicon technology can evolve even in nm technology node. Second is devoted to ferroelectric memories as an ultimate memory solution in many aspects such as lifetime data-retention and endurance; size effects; integration technologies; and feasibility as a fusion memory element. 2. Future memory technology 2.1 Evolution of silicon technology Moore s law It is generally accepted that semiconductor industry will continue to expand rapidly due to steady growth of the mobile, digital consumer and entertainment markets. In addition to these, many more growth engines will appear, encompassing the automotive, informationtechnology, biotechnology, health, robotic and aerospace industries. The advances in silicon technology that has been the backbone of tremendous previous growth, were foreseen in 1965 when Gordon Moore published his famous prediction about the constant growth rate of chip complexity (Moore, 1965). And, in fact, it has repeatedly been shown that the number of transistors integrated into silicon chips has indeed doubled every 18 months. Increases in packing density, according to the Moore s law, are driven by two factors: reductions in production costs and increases in chip performance. Another prominent example of the unstoppable pace of technology advancement 3, has been predicted (Hwang, 2006). Figure 1 shows Moore s doubling phenomena of the number of components the number of gate in case of CPU (central processing unit) and density in memory device. Fig. 1. Moore s doubling phenomena of the number of chips (Moore, 2006). 3Moore s law was predicted to stagnate to the end of the 20th century, but new sources of momentum are able to maintain or acclerate a growth trend. SoC (System-on-a-chip) integration has the potential to continue IC (integrated-circuit) cost reduction and to perpetrate growth of personal Internet products.
4 120 Ferroelectrics - Applications Despite these bright prospects, there is growing concern about whether semiconductor technology can continue to keep pace with demand when silicon technology enters the deep nano-scale dimension. This is because there are limits to transistor scaling, and narrowing margins in manufacturing due to ever-increasing fabrication costs tied to technical complexities (Kim & Jeong, 2005; Kim & Choi, 2006). The manufacturing cost grows because the engineering becomes more complex as transistors shrink in size. The scale is staggering, but the current generation of memory chips is 30 nm node across. This does mean that innovation is more process driven, and may require suppliers to think about what customers need and value, rather than simply pushing for ever greater density of transistors. Though most experts believe that silicon technology will maintain its leadership down to 20 nm, beyond this node a number of fundamental and application-specific obstacles will prevent further shrinkage. A common example is the inevitable occurrence of variations due to rough line edges and surfaces when pattern sizes approach atomic scales (Hwang, 2006). It is therefore the primary aim of this section to present various possible paths to overcome these obstacles and eventually to maintain the technology-scaling trend beyond 20 nm node. As will be shown, these solutions include not only 3-D (three-dimensional) technologies but also non-silicon technologies on a molecular scale. In addition, new applications, and new growth engines for the semiconductor industry will be provided from a combination of separate technologies such as silicon-based IT with new materials (Whang et al., 2003; Wada, 2002). Therefore, this section is structured as follows: First, a review of the evolution of key silicon technologies is given. Next, we discuss scaling limits in each technology node and demonstrate practical and plausible solutions to penetrate these scaling barriers. Both DRAM and NAND flash memory are dealt with in discussion. And then, authors present prospects for the future silicon industry covering fusion technologies Evolution of silicon technology DRAM: Since the first 1,024-bit DRAM was demonstrated by Intel TM in the early 1970 s, the highest available density of DRAM has doubled every 18 months. Now DRAM technology has reached 30 nm in process technology and 4 Gb in density, which will be deployed soon in the marketplace. Further, 20-nm DRAM is being developed at R&D centers around the world. DRAM technology has evolved toward meeting a need for ever-increasing demand both of data retention and of performance improvements. Increases in data retention impose great challenges on DRAM technology by requiring not just a sufficient amount of capacitance in a memory cell but an extremely low level of leakage current from storage junction. As device shrinks, it has been being one of the most challenging to achieve an adequate amount of cell capacitance in DRAM. It is widely agreed that the value of cell capacitance is more than 20 ff, regardless of technology-node migration. This is because sensing signal developed from memory cells, is vulnerable to become interfered by unwanted noise factors according to its operational nature. Sensing signal, Vs can be expressed by equation (1), where C S is cell capacitance at storage node; C BL is parasitic bit-line capacitance; AIVC is cell array internal voltage; and the last term V UN is undesirable noise. In equation (2), the first term I LEAK t REF in the parenthesis is a term of charge loss due to junction leakage current, I JUNC ; gate-induced-drain-leakage (GIDL) current, I GIDL ; and non-generic leakage current, I NG, arising from integration imperfections (e.g., dielectric leakage current and cell-to-cell leakage current) as indicated in equation (3).
5 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 121 All of those loss factors are constituents of data-retention time, so called refresh time, t REF. V N is noise voltage due both to noise coupling and to mis-matches of threshold voltage and conductance of sense amplifiers. Another source of charge loss, Q I in Eq. (2) has to be considered when DRAM is exposed to irradiations such as -particle and cosmic rays. These undesirable components are very difficult to attenuate and become dominant as device dimensions are smaller. To maintain almost non-scalable requirement of cell capacitance of more than 20 ff/cell, dielectric material of cell capacitors have continuously evolved into high-κ dielectric materials and at the same time their structures have been pursued actively for novel ones (Lee et al., 2003a; Kim et al., 2004a). This is due to the fact that cell capacitor area decreases by a factor 4 of 1/k ~ 1/k 2 as technology scales, where k denotes a scaling factor, where k > 1 (See Denard et al., 1974). In general, when designing device to a smaller dimension, the device is scaled by a transformation in three variables: dimension, voltage, and doping concentration. Firstly, all the linear dimensions are reduced by a unit-less scaling constant k, e.g., t OX = t OX /k. Such reduction includes not only vertical dimensions such as thickness of gate oxide and junction depth, but also horizontal dimensions, for example, channel length L and width W. Secondly, voltage applied to the new device has to be reduced by the same factor, e.g., V CC =V CC /k. Lastly, doping concentration, N A is to be increased, e.g., N A = k N A. In practice, DRAM s capacitor has begun with a stacked 2-D (two-dimensional) structure, integrated under bit-line in process architecture 5 until the mid 1990 s. Since then, DRAM has changed in structure to have an integration scheme of cell-capacitors placed over bit-line (COB) though there was an attempt to use trench-type capacitors, which are buried deeply in silicon substrate. In the 1990 s, dielectric material of the cell capacitors has adopted silicon-based dielectrics, SiO 2 /Si 3 N 4, whose dielectric constant lies in between 3.9 and 7.0. With these relatively low-κ dielectrics, a cell capacitor has headed for expanding its area as much as possible. Thus, its structure has been transformed in substantially complex ways, from a simple stack to a hemi-spherical-silicon-grain (HSG) stack, to a HSG cylinder until the late 1990 s. The advent of high-κ dielectrics since the beginning of 21 st century has brought a new era of building the cell capacitors. Table 1 compares fundamental material properties of high-κ candidates with those of conventional low-κ dielectrics. These high-κ dielectrics have allowed us to form the cell capacitors into simpler one-cylinder-stack (OCS) than those in low-κ dielectrics due to relatively higher dielectric constant. Provided high-κ dielectric material utilizes, increase in cell capacitance will be achieved simply by increase in height of a cylinder. Such an increase in height gives rise to skyrocketing of aspect ratio of 4A scaling factor of capacitance C = εa/t is supposed to be 1/k in a 2-D stack structre, but since capacitor thickness t is not a contraint factor any more in a 3-D structure, capacitance can be written in 1/k 2. 5So called capacitor-under-bit-line (CUB) in integration architecture.
6 122 Ferroelectrics - Applications cell capacitors when technology scales, together with dramatic decrease in footprint. In typical, an aspect ratio of cell capacitors ranges from 6 to 9 until 100 nm technology node. A higher aspect ratio has brought another obstacle in building cell capacitors robust: mechanical instability of OCS structures. As a result, many smart engineers in silicon industries has introduced a novel capacitor structure, supporter-added OCS such as mesh type cell capacitors, which can increase the cell capacitor height with desired mechanical stability (Kim et al., 2004a). Taking into account the recent advances of the cell-capacitor technology, the aspect ratio reaches 35 to 45, which is far beyond those of the world tallest skyscrapers, ranging from 8.6 to Materials Dielectric Band gap E G constant (κ) (ev) Crystal Structure(s) SiO Amorphous Si 3 N Amorphous Al 2 O Amorphous Y 2 O Cubic La 2 O Hexagonal, cubic Ta 2 O Orthorhombic TiO Tetragonal, rutile, anatase HfO Monoclinic, tetragonal, cubic ZrO Monoclinic, tetragonal, cubic Table 1. Comparison of material properties of high-κ dielectric candidates with those of conventional low-κ dielectrics (Wilk et al., 2001). In the meanwhile, charging and discharging properties of cell capacitors depend strongly on performance of cell array transistors (CATs). On-current of the CAT plays a critical role in its charging behaviors while off-leakage current of the CAT is a decisive factor to determine their discharging characteristics. On the one hand, on-current (Ion) needs to be at least greater than several 10-6 Ampere to achieve reasonable read and write speed. On the other, off-leakage current (Ioff) has to satisfy a level of Ampere to minimize charge loss just after charging up the cell capacitors to ensure adequate sensing-signal margin as indicated in Eq. (2). Despite continuation of technology migration, the ratio of Ion/Ioff has remained constant to approximately. CAT s technology has evolved to meet this requirement., where µ eff is effective mobility for electrons, C OX is capacitance of gate oxide, W is width of transistor s active dimension, and L eff is effective channel length. At first, from the structural point of view, 2-D planar-type CAT (PCAT) has been moved to 3-D CAT. The reason why 3-D CAT has been adopted is to relieve data retention time. In 100-nm technology node, L eff of the PCATs does not ensure a specific level of off-leakage current requirement (less than A) due to high-field junction. The high electric field is caused by high-doping concentration near the channel region to block short-channel-effect (SCE). Under such a SCE circumstance, a transistor does not, in general, work any longer, by a way of punch-through between source and drain when its channel length becomes shorter. As denoted in Eq. (2) and (3), off-leakage currents I LEAK are closely related to data retention
7 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 123 time. Generically this I LEAK arises from sub-threshold current and gate-induced drain leakage (GIDL) current of cell array transistors along with junction leakage current from storage node. As L eff is scaled down, the increased doping concentration against the SCE strengthens electric field across storage node junction. This increase in junction-leakage current results in degrading the data retention time (Kim et al., 1998). The degradation of data retention time becomes significant below 100 nm node due to rapid increase in junction electric field again (Kim & Jeong, 2005). This issue since the mid 2000 s has been overcome by introducing 3-D cell transistors, where the junction electric-field can be greatly reduced due to lightly doped channel. One example of these newly developed structures is RCAT (Recess Channel Array Transistor) structure whose channel detours around a part of silicon substrate so that the elongated channel can be embodied in the array transistor (Kim et al., 2003). Also, the RCAT structure gives us another benefit, which lessens threshold voltage (Vth) due to lower doping concentration. Thereby, not only does DRAM s core circuitry operate at lower voltage but also CAT s on-current increases, as denoted in Eq. (4). Note that, according to the Moore s law, Vcc must be scaled down for power save. This trend has continued to come to 60 nm technology node. However, beyond 60 nm of technology node, on-current requirement has not been satisfied with such a RCAT approach alone. Thus, further innovations since 50 nm node have been pursued in a way of a negative word-line (NWL) scheme 6 in DRAM core circuitry. The NWL scheme compared with a conventional ground-word-line (GWL) scheme, allows us Vth reduction further, which means more oncurrent. However, another adverse effect on the CAT can occur as a result of the NWL. Since CAT s gate potential goes more negative during holding data stored at the storage junction, from which GIDL current increases as a function of gate-storage voltage, level of which is as high as that of gate potential compared with the conventional GWL. Many device engineers have given much effort to tackle this problem and finally have figured it out by technological implementation, for instance, mitigation of electric field exerted locally in the region overlapped between source/drain and gate in the RCAT. In pursuit of purpose, gate oxide needs to be different in thickness. Provided that the oxide thickness in the overlapped region is thicker than that in the channel, unwanted GIDL current will decrease in proportion to electric field of the overlapped zone in the storage-node to gate (Lee et al., 2008; Jung et al., 2009). According to our calculation, one can extend this NWL-based RCATs down to 40 nm node with minor modifications (Jung et al., 2009). In 30 nm technology node, it becomes extremely difficult to achieve the successful Ion/Ioff ratio. A report has shown that a body-tied FinFET (fin field-effect-transistor) as a cell array transistor seems to be very promising due to its superb performances: excellent immunity against the SCE; high trans-conductance; and small sub-threshold leakage (Lee et al., 2004). For example, it allows us to have not only lower Vth but lower sub-threshold swing due to a fin-gate structure, providing more width for on-current and wrapping the gate for Vth and sub-threshold swing down. It is believed that the body-tied FinFET leads DRAM technology to be extendable down to 30 nm node. In off-leakage current, CAT s gate material has been being transformed to metal gate of higher work function (4.2~4.9 ev) instead of n+ poly-silicon gate. The lower Vth coming from higher work function provides us with lower channel doping. This leads to lower junction electric field and results in lower off-leakage 6Since a level of dc (direct current) bias at unselected word-lines is negative, sub-threshold leakage current of a cell transistor becomes extremely low because its channel has never chance to be on-set of inversion, leading to keeping a reasonable level of off-leakage current despite low Vth.
8 124 Ferroelectrics - Applications current. Figure 2 shows how DRAM s CAT structure has evolved during the past decade. Beyond 30 nm of technology node, a novel structure must be suggested for continuing the successful Ion/Ioff ratio. Among many structures, a vertical channel CAT (VCAT) is one of the good candidates (Yoon et al., 2006). This is because it can plausibly permit us to access an ideal transistor. A VCAT has a surrounding gate buried in silicon substrate (Kim, 2010). Bit-line connected to its data node runs buried under silicon substrate, too. With such a burying architecture, VCAT-base DRAM is expected to provide minimum size of lateral dimension per unit memory element as indicated in the inset of Fig. 2. Fig. 2. Maximum electric field, E MAX as a function of channel-doping concentration in various CAT s structures. As CATs evolves, the doping concentration decreases E MAX, denoted in red in E-field strength of simulation structures as shown in the inset. An example of DRAM architecture based on VCAT is also shown in the insect. NAND flash memory: NAND flash memory has the smallest cell size among silicon-memory devices commercially available due to its simple one transistor configuration per one bit and a serial connection of multiple cells in a string. Because of this, NAND flash has carved out a huge market for itself, as was expected since it first appeared in the mid 1980 s. The need for NAND flash memory will continue to surge due to the recent resurgence of demand for mobile products such as smart phones and smart pads. With the rise of the mobile era, NAND flash has pushed toward ever-higher density, along with improving programming throughput. As a consequence, the memory has evolved toward an ever-smaller cell size in two ways: by increasing string size and by developing two bits per cell, while at the same time, increasing page depth. Now, current NAND flash memory reaches 30 nm node in process technology and 32 Gb in density, mass production of which has blossomed since the late 2000 s. In addition, NAND technology beyond 30 nm is now under development at R&D centers across the world. Alongside the recent development of two-bit-per-cell technology, introduction to multi-bit cells should greatly accelerate this trend.
9 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 125 There are several prerequisite requirements to meet in terms of cell operation. Its cells must satisfy write and read constraints. First is programming disturbance. To program a cell, it is necessary to apply a certain amount of electric field across between floating gate and channel of the cell so that a sufficient amount of Fowler-Nordheim (FN) tunneling electrons can be injected into the floating gate. ~,, where t OX is thickness of tunnel oxide; γ is a coupling ratio; V PGM is programming voltage; C CS is capacitance between control gate and storage media; and C TUNNEL is capacitance of tunnel oxide. Figure 3 illustrates (a) a schematic diagram of NAND cell arrays and (b) their programming conditions. During the programming, there are two types of unselected cells that tolerate unwanted programming: One type is cells connected to the same bit-line of the selected cell. And the other is cells connected to the same word-line. The former suffers so called V PASS -stress cells while the latter endures so called V PGM -stress cells as follows:,, where V PASS stress is voltage applied to the unselected cells which share the same bit-line of the programming cell; V PGM stress is voltage applied to the unselected cells which share the same word-line; and C D is depletion capacitance of silicon substrate (See Fig. 3b). The V PASS - stress and the V PGM -stress are, in general, so small that neither electron injection into the unselected cells nor ejection from those is allowed in programming, respectively. Thus, V PASS window is determined by allowable both V PASS -stress and V PGM -stress. However, the V PASS window will be narrow when scaling down because of increase in depletion capacitance (C D ) as denoted in Eq. (7). Thus, as technology scales, adequate V PASS window has to be satisfied. Next, in read operation, read voltage of a floating gate has to be higher than the highest threshold voltage of a cell string in order to pass read current through the string on which 32 cells are connected in series (in case of Fig. 3a). In similar to programming disturbance, read disturbance might occur in the unselected cells on the same string, and thus together with appropriate pass voltage, it is believed not only to choose tunnel oxide but to regulate its thickness in integration as well. As a rule of thumb, an adequate value of the coupling ratio in read lies in the range of 0.5 ~ 0.6, and reasonable thickness of the tunnel oxide is about 80 Å. Last but not least, one of the fundamental limitations of the NAND flash stems from the number of stored charge because the available number of storage electrons decreases rapidly with technology scaling. Provided that the voltage difference between the nearest states in a 2-level cell is less than 1 V, threshold voltage shifts due to charge loss will be restricted to less than 0.5 V, which puts the limitation on charge loss tolerance as follows, ~.,
10 126 Ferroelectrics - Applications In case of the floating gate, C CS is C ONO of capacitance of oxide-nitride-oxide. Therefore, at most 10% of charge loss is tolerable, which means that less than 10 electrons are only allowed to be lost over a 10 year period. Fig. 3. (a) Schematic diagrams of memory cell arrays and (b) their programming conditions. In technology evolution, flash memory since the late 1990 s has continued to migrate technology node to 70 nm until the beginning of 2000 s, based on a floating gate (FG) (Keeney, 2001; Yim et al., 2003). Due to an unprecedented growing pace of flash-memory demand for use in mobile applications, higher-grade memory in packing density has been driven by burgeoning of multi bits per a cell since the mid 2000 s (Park et al., 2004; Byeon et al., 2005). Now that multi-level cell (MLC) technology means a wide range of V PASS window in Eq. (5) to (7), it is essential to increase the coupling ratio as shown in Eq. (5). In addition, to overcome stringent barrier of charge-loss tolerance is simply to increase storage charge. This can also be achieved by increasing C CS, as indicated in Eq. (9). However, thickness scaling for high C CS may not be easy in case of C ONO (e.g., a floating gate, here). This is because 60-nm flash memory has already reached 13 nm of equivalent oxide thickness (EOT 7 ), which is believed to be a critical limit in thickness, for allowable charge loss ONO thickness ~ 14.5 nm (Park et al., 2004). It has been reported that C CS can be increased by replacing top-blocking oxide into new high-κ dielectric of Al 2 O 3 instead. This provides us with strengthening electric field across the tunnel oxide and at the same time with lessening electric field across the blocking oxide in program and erase. Also, fast erase can be possible even at thicker tunnel oxide of over 30 Å where direct-tunneling hole current could be reduced significantly and thus such a structure gives robust data-retention characteristics (Lee et al., 2005). Meanwhile, from the scaling point of view, flash memories have faced a serious problem since 50 nm of technology node: Cell-to-cell separation becomes so close each other that influence between adjacent cells cannot be ruled out. This is often posed not only by physical aspects of 7EOT indicates how thick a silicon oxide film needs to have the same effect as a different dielectric being used.
11 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 127 cell structures but also by certain aspects of its performance. To circumvent cell-to-cell interference, width of a floating gate tends to be more aggressively squeezed than space between floating gates (See Fig. 3b). This seems to result in a high aspect ratio of a gate stack. Such a high aspect ratio can provoke fabrication difficulty of memory cells due to its mechanical instability. And stored charge (e.g., electron) in a floating gate can redistribute easily in operational conditions, leading to vulnerability of poor data retention. Since the interference originates from another type of coupling between floating gates (FGs), it is desirable to find innovative structures, where charge storage media do not have a form of continuum of charge like the floating gate style but have a discrete sort such as charge traps (CTs) in a nitride layer. The typical examples are non-volatile memories with non-floating gate, for example, SONOS (silicon-oxide-nitride-oxide-silicon) (Mori et al., 1991), SANOS (silicon-alumina-nitride-oxide-silicon) (Lee et al., 2005), TANOS (TaN-alumina-nitride-oxidesilicon) (Shin et al., 2006) or nano-crystal dots (Tiwari et al., 1995; Nakajima et al., 1998). Recently, 32 Gb flash memory has been reported, in particular, in 40 nm of technology node (Park et al., 2006). They have pioneered a novel structure with a high-κ dielectric of Al 2 O 3 as the top oxide and TaN as a top electrode. With this approach, they can achieve several essential properties for NAND flash memory: reasonable programming/erasing characteristics, an adequate V PASS window for multi-bit operation and robust reliability. It is noteworthy that a TANOS structure has much better mechanical stability than that of an FGtype cell because of the far lower stack in height. Interference among TANOS cells hardly occurs due to nature of the charge trap mechanism SiN (silicon nitride) traps act as point charges. This is the biggest advantage in CT-NAND flash memory. To scale NAND flash further down, we may need another cell technology. A FinFET could be a very promising candidate because it can increase storage electrons effectively by a way of expanding channel width of cell transistors, similar to 3-D CATs in DRAM. In this pursuit, a research group has successfully developed flash memory with a TANOS structure based on a 3-D, body-tied FinFET (Lee et al., 2006), where they can obtain excellent performance of NAND-flash cells with robust reliability. If there are much higher κ dielectrics than Al 2 O 3, then we can further scale down the FinFET CT-NAND flash memory. Fig. 4. (a) A schematic diagram of 3-D, body-tied FinFET NAND cells and (b) comparisons of the 3-D cells with 2-D, planar cells in threshold-voltage shift as a function of programmed threshold voltage, measured after suffering 5k program/erase cycles and a bake at 200 C for 2 hours (Lee et al., 2006).
12 128 Ferroelectrics - Applications Figure 4 represents (a) a schematic diagram of 3-D, body-tied FinFET NAND cells and (b) comparisons of the 3-D cells with 2-D ones in threshold-voltage shift as a function of programmed threshold voltage, measured after suffering 5k program/erase cycles and a bake at 200 C for 2 hours. The threshold-voltage delay has been improved to 0.32 V in 3-D NAND cells, compared with 2-D NAND ones. 2.2 Prospects of silicon technology As well aware that the era of 2-D, planar-based shrink technology is coming to an end, semiconductor institutes have seen enormous hurdles to overcome in order to keep up with the Moore s doubling pace and thus to meet the requirements of highly demanding applications in mobile gadgetry. They have attempted to tackle those barriers by smart and versatile approaches of 3-D technology in integration hierarchy. One strand of the responses is to modify structures of elementary constituents such as DRAM s CATs, its storage capacitors and storage transistors of flash memory to 3-D ones from the 2-D. A second thread revisits these modifications to a higher level of integration: memory stacking. And another move is to upgrade this into a system in a way of fusing of each device in functionality by utilizing smart CMOS technology, e.g., through-silicon-via (TSV) Elementary level of 3-D approach When working with silicon devices, a transistor s key parameters must take into account: on-current; off-leakage current; the number of electrons contained in each transistor; or the number of transistors integrated. All of these factors are very important, but not equally important in functional features of silicon devices. For instance, for memory devices, offleakage current is regarded as a more important factor and thus memory technologies tend to be developed with a greater emphasis on reducing off-leakage current. For logic, transistor delay is the single most important parameter, not just to indicate chip performance but to measure a level of excellence in device technology as well. This transistor delay is related closely to transistor s on-current state. And with 2-D planar technology in logic, one can continue to reduce transistor s channel length down to 40 nm. However, at less than 30 nm, the transistor begins to deviate in spite of a much relaxed offcurrent requirement. This is because of non-scalable physical parameters such as mobility, sub-threshold swing and parasitic resistance. To resolve these critical issues, two attempts have been examined. One is to enhance carrier mobility by using mobility-enhancement techniques such as strained silicon (Daembkes et al., 1986), SiGe/Ge channel (Ghani et al., 2003), or an ultra thin body of silicon (Hisamoto et al., 1989), where carrier scattering is suppressed effectively. Another approach is to reduce channel resistance by widening transistor s width. In this case, it appears very promising to use different channel structures such as tri-gate (Chau et al., 2002) or multi channel (Lee et al., 2003b). We have witnessed that, with 3-D FinFETs in memory devices, this attempt is very efficient for extending incumbent shrink technology down to 30 nm of technology node. As silicon technology scales down further, the two will eventually be merged into one single solution for an optimum level of gate control. With this type of structure, one will arrive at nearly ideal transistor performance such as being virtually free from the SCE, sufficient on-current and suppressed off-leakage current. Figure 5 shows (a) evolution trends of logic transistors in terms of EOT: A sharp decrease in EOT trend appears due to lack of gate controllability in 2- D planar structures despite high-κ dielectrics. By contrast, those in 3-D, multi-gate structures
13 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 129 are expected to have the same trend of EOT as those with conventional SiON dielectrics. This suggests that 3-D structures seem to become essential even with high-κ materials. It is thus believed that developing a 3-D transistor with either a multi-gate or an gate-all-around structure (Colinge et al, 1990) is quite feasible if one can extend 2-D planar technology to 3- D. This is because the channel length is no longer restricted by lateral dimension. Figure 5 also shows (b) a cross-sectional TEM (transmission-electron-micrograph) image of one of the 3-D, multi-gate transistors and (c) its Ion-Ioff characteristics are compared with those of 2-D planar structures. Fig. 5. (a) Equivalent-oxide-thickness (EOT) scaling trends (Kim, 2010) are shown in reciprocal scale. Due to the difficulty in controlling the SCE, a sharp decrease in EOT trend is inevitable for the coming nodes. However, the historical trend can be reverted back in the case of 3-D, multi-gate transistors. (b) A cross-sectional TEM image of a 3-D, multi-gate and (c) its Ion-Ioff characteristics are compared with those of the planar (Lee et al., 2003b) D stacking of memory cells New silicon technology based on 3-D integration has drawn much attention because it seems to be regarded as one of the practical solutions. Though the concept of 3-D integration was first proposed in the early 1980 s (Kawamura et al., 1983; Akasaka & Nishimura, 1986), it has never been thoroughly investigated or verified until now, as neither silicon devices approached their limits at those times nor high-quality silicon crystal was ready for fabrication. Recent advances both in selective epitaxial silicon growth at low temperature (Neudeck et al., 2000) and in high quality layer-transferring technology with high-precision processing (Kim et al., 2004b), can bring major new momentum to the silicon industry via 3- D integration technology. The simplicity of memory architecture consisting of memory array, control logic and periphery logic, makes it relatively easy to stack one-memory cell array over another. This will ultimately lead to multiple stack designs of many different memories. Recently, one of the memory manufacturers has started to implement 3-D integration technology with SRAM to reduce large cell-size (Jung et al., 2004). Figure 6
14 130 Ferroelectrics - Applications shows (a) a cross-sectional TEM image of 3-D stacking SRAM (Left) and its schematic diagram (Right) (Jung et al., 2004): Since transistors stacked onto a given area do not need to isolate p-well to n-well, SRAM-cell size of 84 F 2 is being reduced to the extremely small cell size of 25 F 2. Encouraged by this successful approach, stacked flash memory has also been pursued. Figure 6 also represents (b) 3-D stacking NAND flash memory (Jung et al., 2006): This suggests great potential of 3-D memory stacking for large-scale use with 3-D flash-cell technology, which will spur further growth in high-density applications. Beyond 20 nm node, we believe that the most plausible way to increase density is to stack the cells vertically. Figure 6 displays (c) a 3-D schematic view of vertical NAND flash memory (Katamura et al., 2009), where SG is selecting gate, CG is control gate and PC is pipe connection. The stacking of memory cells via 3-D technology looms on the horizon, in particular, for NAND flash memory. Fig. 6. (a) A cross-sectional TEM image of 3-D stacking SRAM (Left) and its schematic diagram (Right) (Jung et al., 2004). (b) 3-D stacking NAND flash memory (Jung et al., 2006). (c) A 3-D schematic view of vertical NAND flash memory (Katsumata et al., 2009), where SG is selecting gate; CG is control gate; and PC is pipe connection. (d) A cross-sectional SEM image of memory array after the removal of the sacrificial film (See Katsumata et al., 2009) It is also believed that logic technology will shift to 3-D integration after a successful jumpstart in silicon business. The nature of a logic device, where transistors and interconnections are integrated as key elements, is not much different from those of stacked memory cells. It may be very advantageous to introduce 3-D integration technology to a logic area. Note that implementation of interconnection processes seems to be more efficient in vertical scale. For example, a dual or quad-core CPU can be realized with only a half or quarter of the chip size, which will result in significantly greater cost-effectiveness. Another promising use would be to improve logic performance by cutting down on the length of metallization. Decrease in interconnection length means a huge amount of reduction in parasitic RC components, i.e., a high speed and power saving. In addition, 3-D technology will make it easy to combine a memory device and a logic device onto one single chip
15 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 131 through hierarchical stacking. Since most parts of SoCs (system-on-chips) in the future will be allocated to memory, this combining trend will be accelerated. The next step will be to stack multi-functional electronics such as RF (radio frequency) modules, CISs (CMOS image sensors) and bio-sensors over the logic and memory layers Chip level of 3-D integration The early version of 3-D integration in chip level has been commercialized already in a multi-chip package (MCP), where each functional chip (not device) is stacked over one another and each chip is connected by wire bonding or through the through-via hole bonding method within a single package. Figure 7 exhibits (a) a bird s eyes view of multichip-package (MCP) by wire bonding; (b) wafer-level stack package with through-via-hole; (c) a photograph of 3-D integrated circuit; and (d) a schematic drawing of a 3-D device for use in medical applications. The advantages of the MCP are a small footprint and better performance compared to a discrete chip solution. It is expected that the MCP approach will continue to evolve. However, the fundamental limitation of MCP will be lack of costeffectiveness due to a number of redundancy/repair requirements. In this respect, throughsilicon-via (TSV) technology is able to overcome MCP limitations through an easy implementation of redundancies and repairs. Many groups have reported TSV-based integrated circuit (TSV IC), where a single integrated circuit is built by stacking silicon wafers or dies and interconnecting them vertically so that they can function as one single device (Topol et al., 2006; Arkalgud, 2009; Chen et al., 2009). In doing so, key technologies include TSV formation, wafer-thinning capability, thin wafer handling, wafers backside processes, and 3D-stacking processes (e.g., die-to-die, die-to-wafer and wafer-to-wafer). In detail, there are many challenging processes such as etching profiles of TSV sidewall, poor isolation liners and barrier-deposition profiles. All of these are likely to provoke TSV s reliability concerns due to lack of protection from metal (e.g., Cu) contamination. A report of silicon-based TSV interposers (Rao et al., 2009) may have advantages over traditional PCB or ceramic substrate in that it has a shorter signal routing. This results from vertical interconnect and improved reliability due to similarity to silicon-based devices in thermal expansion and extreme miniaturization in volume. TSV-IC technologies together with the 3- D interposers will accelerate an adoption of 3-D system-in-package (SiP) with heterogeneous integration (See Fig. 7d). And this might be a next momentum for genuine 3D IC devices in the future because of tremendous benefits in footprint, performance, functionality, data bandwidth, and power. Besides, as the use of 3-D silicon technology has great potential to migrate today s IT devices into a wide diversification of multi-functional gadgetry, it can also stimulate a trend that merges one technology with another, ranging from new materials through new devices to new concepts. In this regard, new materials may cover the followings: carbon nano-tube (CNT) (Iijima, 1991), nano-wire (NW) (Yanson et al., 1998), conducting polymer (Sirringhaus et al. 1998), and molecules (Collier et al., 1999). New devices could also be comprised of many active elements, such as tunneling transistors (Auer et al., 2001), spin transistors (Supriyo Datta & Biswajit Das, 1990), molecular transistors (Collier et al., 1999), single electron transistors (SETs) (Fulton & Dolan, 1987) and others. We may be able to extend this to new concepts, varying from nano-scale computing (DeHon, 2003) and FET decoding (Zhong et al., 2003) to lithography-free addressing (DeHon et al., 2003). To a certain extent, some of these will be readily integrated with 3-D silicon technologies. This integration will further enrich 3-D silicon technologies to create a variety of new multifunctional electronics, which will provide further substantive boosts to silicon industry, allowing us to make a projection of a nano-silicon era into practical realities tomorrow.
16 132 Ferroelectrics - Applications Fig. 7. (a) A bird s eyes view of (a) multi-chip-package (MCP) by wire bonding. (b) Waferlevel stack package with through-via-hole. (c) A Photograph of 3-D integrated circuit. (d) A schematic drawing of a 3-D device for medical applications enabled by TSVs and silicon interposers. These realities will be manifested in highly desirable applications of combining of information technology (IT), bio-technology (BT), and nano-technology (NT), to become so called fusion technology (FT). Given that key obstacles to realize this are tackled by bridging the gap between previously incompatible platforms in silicon-based CMOS technology and new technological concepts, a vast number of new applications will unfold. One example may be many applications related to health sensor technology, in particular, the early recognition of cancer diseases and the screening of harmful and poisonous elements pervasive in the environment. Further, when a nano-scale bio-transistor is available, lab-on-a-chip (LoC) will become a single solution integrating all of its essential components, such as micro-array, fluidics, sensors, scanners and displayers. Then, by its very nature 8, one will have tons of benefits from a mass of disposable LoCs, which will stimulate the future silicon industry. 8As a successful booster for the silicon industry, whatever will be, it should be a high volume product at a reasonable price. PCs are high volume products, and hand-held phones are too. In that sense, LoC is very promising because its potential market is the entire population.
17 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution Remarks Not only do many challenges await silicon industries as technology enters the deep nanodimension era but promising opportunities are also there. Equipped with new technologies such as 3-D scaling and a wealth of new materials, alongside fusing of related technologies, we will overcome many hurdles ahead and respond technological challenges we will stumble along the way. All plausible solutions described earlier tell us that planar-based technology will reach an impassable limit. 3-D technology begins to provide clear signs of serving as a foundation for a refuel of the silicon industry. The advantages of 3-D integration are numerous. They include: elimination of uncertainty in the electrical characteristics of deep nano-scale transistors; extendable use of silicon infrastructures, especially optical lithography tools; and formation of a baseline for multi-functional electronics and thus facilitation of implementing a hierarchical architecture, where each layer is dedicated to a specific functional purpose. Over the next decade, we will see great endeavors in numerous areas that will greatly stimulate the semiconductor business. Successful evolutions of device structures will continue and even accelerate at a greater pace in the not-too-distant future. In addition, device designs will converge onto a single mobile platform, covering many different capacities and services from telecommunication through broadcasting and a much higher degree of data processing. In line with this, silicon technology will still play a critical role in realizing functionally merged solutions. All of these will permit us to have invaluable clues not just on how to prepare future silicon technology but also on how to positively influence the entire silicon industry. This will allow us to attain an even more sophisticated fusing of technologies. As seen in the past, silicon technology will continue to provide our society with versatile solutions and as-yet unforeseen benefits in much more cost-effective ways. 3. Ferroelectric memory as an ultimate memory solution 3.1 Introduction There has been great interest to understand ferroelectric properties from the point of view of both fundamental physics and the need of nano-scale engineering for memory devices. On the one hand, since electric hysteresis in Rochelle salt was in 1920 discovered by Valasek (Valasek, 1921), there have been tremendous efforts to look through ferroelectricity in a comprehensive way over the past many decades. As a consequence, the phenomenological theory of ferroelectricity has been presented by many researchers: Devonshire (Devonshire, 1949; Devonshire, 1951); Jona and Shirane (Jona and Shirane, 1962); Fatuzzo and Merz (Fatuzzo and Merz, 1959); Line and Glass (Line and Glass, 1979); and Haun (Haun, 1988). The series of their works have been successful to express the internal energy of a ferroelectric crystal system. This theory has also been examined experimentally in detail, and extended by Merz (Merz, 1953); by Drougard et. al. (Drougard et al., 1955); and by Triebwasser (Triebwasser, 1956). Especially, Devonshire s phenomenological theory (Devonshire, 1949; Devonshire, 1951) gives the free energy of BaTiO 3 as a function of polarization and temperature. From this free energy we know what the possible state and meta-stable states of polarization are in the absence of an applied field. We also know how polarization changes as a function of field applied to the crystal. In short, according to the theory, a ferroelectric possesses two minima (e.g., a second-order phase transition) in the internal energy. These two minima are separated by an energy barrier ΔE. Essential feature of a ferroelectric is that these two minima corresponds to two different spontaneous
18 134 Ferroelectrics - Applications polarizations that can be changeable reversibly by an applied field. Under an assumption that applied electric field is able to surmount the energy barrier, the advent of smart thinfilm technology in evolution of CMOS technology, has enabled to consider a ferroelectric crystal a useful application. Thinning a ferroelectric film with high purity means that there could be an opportunity to use ferroelectrics as a memory element. On the other, integrated ferroelectrics are a subject of considerable research efforts because of their potential applications as an ultimate memory device due to 3 reasons: First, the capability of ferroelectric materials to sustain an electrical polarization in the absence of an applied field, means that integrated ferroelectric capacitors are non-volatile. They can retain information over a long period of time without a power supply. Second, the similar architectural configuration of memory cell-array to conventional ones, means that they are highly capable of processing massive amounts of data. Finally, nano-second speed of domain switching implies that they are applicable to a high-speed memory device. Since ferroelectric capacitors was explored for use in memory applications by Kinney et al. (Kinney et al., 1987); Evans and Womack (Evans & Womack, 1988); and Eaton et al. (Eaton et al., 1988), it has been attempted to epitomize ferroelectrics to applicable memory solutions in many aspects. In the beginning of 1990 s, silicon institutes have begun to exploit ferroelectrics as an application for high-density DRAMs (Moazzami et al., 1992; Ohno et al., 1994). This is because permittivity of ferroelectrics is so high as to achieve DRAM s capacitance extremely high and thus appropriate for high density DRAMs. An early version of non-volatile ferroelectric RAM (random-access-memory) used to be several kilo bits in packing density. This lower density (NB. at that moment, DRAM had several ten mega bits in density) is because of two: One is that its memory unit was relatively large in size, being comprised of two transistors and two capacitors (2T2C) to maximize sensing signal. The other is that a ferroelectric capacitor stack has required not only novel metal electrodes such as platinum, iridium and rhodium, all of which are hard to be fine-patterned due to processing hardness, but also reluctant metal-oxide materials to conventional CMOS integration due to possible cross contaminants such as lead zircornate titanate (PbZrTiO 3 ) and strontium bismuth titanate (Sr 1-x Bi x TiO 3 ). Next steps for high density non-volatile memory have been forwarded (Tanabe et al., 1995; Sumi et al., 1995; Song et al., 1999). In similar to DRAM, an attempt to build smaller unit cell in size was in the late 1990 s that one transistor and one capacitor (1T1C) per unit memory was developed (Jung et al., 1998). Since then, many efforts to build high density FRAM have been pursued, leading to several ten mega bits in density during the 2000s (Lee et al., 1999; Kim et al., 2002; Kang et al., 2006; Hong et al., 2007; Jung et. al, 2008). Fig. 8. (a) Evolution of electronic components in data throughput performance. (b) NVM (non-volatile memory) filling price/performance gap.
19 Future Memory Technology and Ferroelectric Memory as an Ultimate Memory Solution 135 Among integrated ferroelectrics, one of the most important parameters in FRAM is sensing signal margin. The sensing signal of FRAM is proportional to remanent polarization (P r ) of a ferroelectric capacitor as follows:, where A is capacitor s area; d is capacitor s thickness. As seen in equation (10), in principle, we have to compensate the area reduction when technology scales down. However, in practice, when the thickness of PZT ferroelectric thin film decreases, degradation of polarization tends to appear in the ferroelectric capacitor due to a dead layer between the ferroelectric and electrodes (See section 3.3.3). Unlike the requirement of DRAM s CAT, the array transistor of FRAM is not necessarily constrained from the off-leakage current due to no need of the refresh cycles, but from on-current, which is at least greater than several µa in order for a reasonable read and write speed. Thus, this will greatly relieve technology scaling quandaries and enable fast technology migration to the high end. This is because designing of a less leaky cell transistor becomes very difficult in incumbent memories such as DRAM and NAND/NOR flash due to need of lower doping concentration. As witnessed in the Moore s law, there has been enormous improvement in VLSI (very large-scale integration) technology to implement system performance of computing platforms in many ways over the past decades. For instance, data throughput of central processing unit (CPU) has been increased by thousand times faster than that of Intel 286 TM emerged in the beginning of 1980 s. Alongside, a latest version of DRAM reaches a clock speed of more than 1 GHz. By contrast, state-of-the-art HDD (hard disk drive) transfers data at 600 MB/sec around (See Fig. 8a). Note that data rate of the latest HDD is still orders of magnitude slower than the processor/system-memory clock speed (see Fig. 8b). To achieve the throughput performance in more effective way, it is therefore needed to bridge performance gap in between each component. To compensate the gap between CPU and system memory, a CPU cache 9 has been required and adopted. In line with this, ferroelectric memory is non-volatile, high-speed. But it has a destructive read-out scheme in core circuitry, whose memory cells need to return the original state after being read. This is because the original information is destroyed after read. As a result, it is essential to return the information back to its original state, which is so-called restore, necessarily following the read. This operation is so inevitable in the destructive read-out memory such as DRAM and FRAM. In particular, when the ferroelectric memory are used as one of the storage devices in computing system, such as a byte-addressable non-volatile (NV)-cache device, the memory has to ensure lifetime endurance, which is regarded as the number of read/write (or erase if such operation is required) cycles that memory can withstand before loss of any of entire bit information. Thus, authors are here trying to attempt not only how FRAM provides NV-cache solutions in a multimedia storage system such as solid state disk (SSD) with performance benefits but also what should be satisfied in terms of lifetime dataretention and endurance in such applications. Here, we also put forward size effect of ferroelectric film in terms of temperature-dependent dielectric anomaly because a dead layer plays an adverse role in thickness scaling. In addition, it is very important to ensure that integration technology of FRAM in nano-dimension is extendable to one of the 9File system cache is an area of physical memory that stores recently used data as long as possible to permit access to the data without having read from the disk.
20 136 Ferroelectrics - Applications conventional memories. Accordingly, we will present key integration technologies for ferroelectric memory to become highly mass-productive, highly reliable and highly scalable. This covers etching technology to provide a fine-patterned cell with less damage from plasma treatments; stack technology to build a robust ferroelectric cell capacitor; encapsulation technology to protect the ferroelectric cell capacitors from process integration afterwards; and vertical conjunction technology onto ferroelectric cell capacitors for multilevel metallization processes. 3.2 Non-volatile RAM as an ultimate memory solution SSD, one of the multimedia storage systems, in general, consists of 4 important devices. First is a micro-controller having a few hundreds of clock speed in MHz, with real-time operating system (firmware). Second is solid-state storage device such as HDD or NAND flash memory, which has several hundreds of memory size in gigabyte. Third is host interface that has the primary function of transferring data between the motherboard and the mass storage device. In particular, SATA (serial advanced technology attachment) 6G (6 th generation) offers sustainable 100 MB/s of data disk rate in HDD. In addition, bandwidth required in DRAM is dominated by the serial I/O (input/output) ports whose maximum speed can reach 600 MB/s. SATA adapters can communicate over a high-speed serial cable. Last is a buffer memory playing a considerable role in system performance. As such, DRAM utilization in SSD brings us many advantages as a buffer memory. For example, in DRAMemployed SSD, not only does I/O shaping in DRAM allow us to align write-data unit fitted into NAND flash page/block size but collective write could also be possible. As a result of sequential write, the former brings a performance benefit improved by 60% at maximum, and also the latter gives us another performance benefit improved by 17% due to increase in cache function, as shown in Fig. 9a and b, respectively. Fig. 9. Impact of DRAM utilization in SSD on system performance. (a) Increase in sequential read/write by I/O shaping. (b) Performance improvement by collective WRITE. (c) Additional performance benefit for DRAM plus FRAM in SSD. As an attempt to implement system performance further, not only does DRAM have been considered but FRAM has also been taken into account because of its non-volatility and random accessibility. Before that, it is noteworthy that, in SSD with no NV-cache, system-log manager is needed to record and maintain log of each transaction 10 in order to ensure that 10Each set of operations for performing a specific task.
White Paper Implementation Of High-k/Metal Gates In High-Volume Manufacturing INTRODUCTION There have been significant breakthroughs in IC technology in the past decade. The upper interconnect layers of
Order this document by /D Non-Volatile Memory Technology Overview By Stephen Ledford Non-Volatile Memory Technology Center Austin, Texas Introduction Today s microcontroller applications are more sophisticated
Static-Noise-Margin Analysis of Conventional 6T SRAM Cell at 45nm Technology Nahid Rahman Department of electronics and communication FET-MITS (Deemed university), Lakshmangarh, India B. P. Singh Department
Samsung 2bit 3D V-NAND technology Gain more capacity, speed, endurance and power efficiency Traditional NAND technology cannot keep pace with growing data demands Introduction Data traffic continues to
SLC vs MLC: Proper Flash Selection for SSDs in Industrial, Military and Avionic Applications A TCS Space & Component Technology White Paper Introduction As with most storage technologies, NAND Flash vendors
Samsung emcp Samsung Multi-Chip Packages can help reduce the time to market for handheld devices WLI DDP Package Deliver innovative portable devices more quickly. Offer higher performance for a rapidly
Table of Contents Preface Acknowledgements Chapter 1: Overview 1.1 Silicon on Insulator a brief Introduction 1.2 Circuits and SOI 1.3 Technology and SOI Chapter 2: SOI Materials 2.1 Silicon on Heteroepitaxial
Intel s Revolutionary 22 nm Transistor Technology Mark Bohr Intel Senior Fellow Kaizad Mistry 22 nm Program Manager May, 2011 1 Key Messages Intel is introducing revolutionary Tri-Gate transistors on its
SLC vs MLC: Which is best for high-reliability apps? Here's an examination of trade-offs, with an emphasis on how they affect the reliability of storage targeted at industrial, military and avionic applications.
Yaffs NAND Flash Failure Mitigation Charles Manning 2012-03-07 NAND flash is one of very few types of electronic device which are knowingly shipped with errors and are expected to generate further errors
Nanotechnologies for the Integrated Circuits September 23, 2015 Dr. Bertrand Cambou Professor of Practice NAU, Cybersecurity School of Informatics, Computing, and Cyber-Systems Agenda The Market Silicon
3D NAND Technology Implications to Enterprise Storage Applications Jung H. Yoon Memory Technology IBM Systems Supply Chain Outline Memory Technology Scaling - Driving Forces Density trends & outlook Bit
9 ROM, EPROM, & EEPROM TECHNOLOGY Overview Read only memory devices are a special case of memory where, in normal system operation, the memory is read but not changed. Read only memories are non-volatile,
DESIGN CHALLENGES OF TECHNOLOGY SCALING IS PROCESS TECHNOLOGY MEETING THE GOALS PREDICTED BY SCALING THEORY? AN ANALYSIS OF MICROPROCESSOR PERFORMANCE, TRANSISTOR DENSITY, AND POWER TRENDS THROUGH SUCCESSIVE
10 FLASH TECHNOLOGY Overview Flash memory technology is a mix of EPROM and EEPROM technologies. The term flash was chosen because a large chunk of memory could be erased at one time. The name, therefore,
Electronics Field-effect transistors Prof. Márta Rencz, Gergely Nagy BME DED October 7, 2013 The basics of field-effect transistors The operation of field-effect transistors is based on ability of controlling
SLC vs MLC NAND and The mpact of Technology Scaling White paper CTWP010 Cactus Technologies Limited Suite C, 15/F, Capital Trade Center 62 Tsun Yip Street, Kwun Tong Kowloon, Hong Kong Tel: +852-2797-2277
International Journal of Engineering and Technical Research (IJETR) ISSN: 2321-0869, Volume-2, Issue-6, June 2014 Technical Summary on Non-Volatile ROMs Sampa Paul Abstract In this paper, several types
3D GPU ARCHITECTURE USING CACHE STACKING: PERFORMANCE, COST, POWER AND THERMAL ANALYSIS Ahmed Al Maashri, Guangyu Sun, Xiangyu Dong, Vijay Narayanan and Yuan Xie Department of Computer Science and Engineering,
Chapter 9 Semiconductor Memories Jin-Fu Li Department of Electrical Engineering National Central University Jungli, Taiwan Advanced Reliable Systems (ARES) Lab. Jin-Fu Li, EE, NCU 2 Outline Introduction
Ferroelectric Field Effect Transistors Reza M. Rad UMBC Based on pages 387-403 of Nanoelectronics and Information Technology,, Rainer Waser Introduction Ferroelectrics: : dielectric crystals which show
Construction Analysis Winbond W2E512/W27E257 EEPROM Report Number: SCA 9703-533 Global Semiconductor Industry the Serving Since 1964 15022 N. 75th Street Scottsdale, AZ 85260-2476 Phone: 602-998-9780 Fax:
CONTENTS Preface. Energy Band Theory.. Electron in a crystal... Two examples of electron behavior... Free electron...2. The particle-in-a-box approach..2. Energy bands of a crystal (intuitive approach)..3.
Module 3 : Fabrication Process and Layout Design Rules Lecture 12 : CMOS Fabrication Technologies Objectives In this course you will learn the following Introduction Twin Well/Tub Technology Silicon on
Designed for broadband commercial and military applications using push pull circuits at frequencies to 500 MHz. The high power, high gain and broadband performance of these devices makes possible solid
Module 2 Embedded Processors and Memory Version 2 EE IIT, Kharagpur 1 Lesson 5 Memory-I Version 2 EE IIT, Kharagpur 2 Instructional Objectives After going through this lesson the student would Pre-Requisite
CHAPTER IV Multilevel Charge Storage in Silicon nanocrystal Multilayers 4.1 The concept of multi-bit/cell Recent performance improvements in products such as mobile phones, laser printers, and GPS systems
Winbond W971GG6JB-25 1 Gbit DDR2 SDRAM 65 nm CMOS DRAM Process Process Review For comments, questions, or more information about this report, or for any additional technical needs concerning semiconductor
Intel Broadwell SR217 Core M-5Y10 Microprocessor Structural Analysis 1891 Robertson Road, Suite 500, Ottawa, ON K2H 5B7 Canada Tel: 613-829-0414 chipworks.com Structural Analysis 2 Some of the information
Intel Labs at ISSCC 2012 Copyright Intel Corporation 2012 Intel Labs ISSCC 2012 Highlights 1. Efficient Computing Research: Making the most of every milliwatt to make computing greener and more scalable
Ultra-High Density Phase-Change Storage and Memory by Egill Skúlason Heated AFM Probe used to Change the Phase Presentation for Oral Examination 30 th of May 2006 Modern Physics, DTU Phase-Change Material
White Paper Crossbar Resistive Memory: The Future Technology for NAND Flash By Hagop Nazarian, Vice President of Engineering and Co-Founder Abstract NAND Flash technology has been serving the storage memory
Office of the Secretary of Defense National Aeronautics and Space Administration Long Term Data Retention of Flash Cells Used in Critical Applications Keith Bergevin (DMEA) Rich Katz (NASA) David Flowers
ECE 410: VLSI Design Course Introduction Professor Andrew Mason Michigan State University Spring 2008 ECE 410, Prof. A. Mason Lecture Notes Page i.1 Age of electronics microcontrollers, DSPs, and other
Introduction to Organic Electronics (Nanomolecular Science Seminar I) (Course Number 420411 ) Fall 2005 Organic Field Effect Transistors Instructor: Dr. Dietmar Knipp Information: Information: http://www.faculty.iubremen.de/course/c30
Field Effect Transistors (FETs) utilize a conductive channel whose resistance is controlled by an applied potential. 1. Junction Field Effect Transistor (JFET) In JFETs a conducting channel is formed of
Our Embedded Dream of the Invisible Future Since the invention of semiconductor chips, the evolution of mankind s culture, society and lifestyle has accelerated at a pace never before experienced. Information
Optimization for SEU/SET Immunity on 0.15 mm Fully Depleted CMOS/SOI Digital Logic Devices A. Makihara H. Asai Y. Tsuchiya Y. Amano M. Midorikawa H. Shindou S. Kuboyama S. Onoda T. Hirao Y. Nakajima Y.
New Ferroelectric Material for Embedded FRAM LSIs V Kenji Maruyama V Masao Kondo V Sushil K. Singh V Hiroshi Ishiwara (Manuscript received April 5, 2007) The strong growth of information network infrastructures
CS257 Introduction to Nanocomputing Overview of Crossbar-Based Computing John E Savage Overview Intro to NW growth methods Chemical vapor deposition and fluidic assembly Nano imprinting Nano stamping Four
Power-Saving Techniques and Future Design of SPARC64 V/VI V Aiichiro Inoue (Manuscript received May 31, 2007) The performance of high-end microprocessors has increased along with improvements in semiconductor
Making of a Chip Illustrations 22nm 3D/Trigate Transistors Version January 2012 1 The illustrations on the following foils are low resolution images that visually support the explanations of the individual
Packaging - Enabler for Integration in Mobile Applications Andreas Wolter Mobile and Communications Group June 27 th, 2013 Content Mobile and Communications Group Mobile Evolution System Integration Chip/
DEVELOPMENTS & TRENDS IN FEOL MATERIALS FOR ADVANCED SEMICONDUCTOR DEVICES Michael Corbett firstname.lastname@example.org Semicon Taiwan2015 LINX BACKGROUND Linx Consulting 1. We help our clients to succeed
The MOSFET Introduction Metal oxide semiconductor field effect transistor (MOSFET) or MOS is widely used for implementing digital designs Assets: High integration density and relatively simple manufacturing
Lecture Outline Computer/Data Storage Technology Objectives Describe the distinguishing characteristics of primary and secondary storage Describe the devices used to implement primary storage Compare secondary
Ultra Low Profile Silicon Capacitors (down to 80 µm) applied to Decoupling Applications. Results on ESR/ESL. Laurent Lengignon, Laëtitia Omnès, Frédéric Voiron IPDiA, 2 rue de la girafe, 14000 Caen, France
3D Charge Trapping (CT) NAND Flash Yen-Hao Shih Macronix International Co., Ltd. Hsinchu,, Taiwan Email: email@example.com 1 Outline Why Does NAND Go to 3D? Design a 3D NAND Flash Memory Challenges and
Abstract Flash memory used for mass data storage has supplanted the photographic film and floppy disk markets. It has also largely replaced the use of magnetic tape, CD, DVD and magnetic hard disk drives
1. Memory technology & Hierarchy RAM types Advances in Computer Architecture Andy D. Pimentel Memory wall Memory wall = divergence between CPU and RAM speed We can increase bandwidth by introducing concurrency
Alpha CPU and Clock Design Evolution This lecture uses two papers that discuss the evolution of the Alpha CPU and clocking strategy over three CPU generations Gronowski, Paul E., et.al., High Performance
Nanocomputer & Architecture Yingjie Wei Western Michigan University Department of Computer Science CS 603 - Dr. Elise dedonckor Febrary 4 th, 2004 Nanocomputer Architecture Contents Overview of Nanotechnology
03 Basics Understanding the Technology Behind Your SSD Although it may all look the same, all is not created equal: SLC, 2-bit MLC, 3-bit MLC (also called TLC), synchronous, asynchronous, ONFI 1.0, ONFI
Module 7 : I/O PADs Lecture 33 : I/O PADs Objectives In this lecture you will learn the following Introduction Electrostatic Discharge Output Buffer Tri-state Output Circuit Latch-Up Prevention of Latch-Up
Technical Guide Programming NAND devices Kelly Hirsch, Director of Advanced Technology, Data I/O Corporation Recent Design Trends In the past, embedded system designs have used NAND devices for storing
How to Improve Tablet PCs and Other Portable Devices with MEMS Timing Technology The tremendous success of tablets and smart phones such as the ipad, iphone and Android based devices presents both challenges
Hironori Akiba Satoshi Fukuhara Ken-ichi Bandou Hidetoshi Fukuda As the thinning of semiconductor device progresses more remarkably than before, uniformity within silicon wafer comes to be strongly required
CCD Image Sensor Noise Sources Image Sensor Solutions Eastman Kodak Company Rochester, New York 14650-2010 August 8, 2001 Revision 1 Introduction: In an ideal digital camera, the noise performance is limited
Continuous-Time Converter Architectures for Integrated Audio Processors: By Brian Trotter, Cirrus Logic, Inc. September 2008 As consumer electronics devices continue to both decrease in size and increase
2009 International Symposium on Computing, Communication, and Control (ISCCC 2009) Proc.of CSIT vol.1 (2011) (2011) IACSIT Press, Singapore An Open Architecture through Nanocomputing Joby Joseph1and A.
Chapter 1 Introduction to The Semiconductor Industry 1 The Semiconductor Industry INFRASTRUCTURE Industry Standards (SIA, SEMI, NIST, etc.) Production Tools Utilities Materials & Chemicals Metrology Tools
Pervasive Power: Integrated Energy Storage for POL Delivery Pervasive Power Overview This paper introduces several new concepts for micro-power electronic system design. These concepts are based on the
Large-Capacity Flash Memories and Their Application to Flash Cards 68 Large-Capacity Flash Memories and Their Application to Flash Cards Takashi Totsuka Kazunori Furusawa OVERVIEW: Flash cards using flash
Providing Battery-Free, FPGA-Based RAID Cache Solutions WP-01141-1.0 White Paper RAID adapter cards are critical data-center subsystem components that ensure data storage and recovery during power outages.
R. Fontana¹, G. Decad¹, S. Hetzler² ¹IBM Systems Technology Group, ²IBM Research Division 20 September 2012 Technology Roadmap Comparisons for TAPE, HDD, and NAND Flash: Implications for Data Storage Applications
Overview This document describes basic synchronous SRAM operation, including some of the most commonly used features for improving SRAM performance. Fast, Faster, Fastest As microprocessors and other electronics
I-Temp SSDs: Temperature Considerations for Industrial Embedded SSDs NAND flash-based SSDs and memory cards continue to be the dominant storage media for most industrial-embedded systems. Historically,
Data Distribution Algorithms for Reliable Parallel Storage on Flash Memories Zuse Institute Berlin November 2008, MEMICS Workshop Motivation Nonvolatile storage Flash memory - Invented by Dr. Fujio Masuoka
Thin Is In, But Not Too Thin! K.V. Ravi Crystal Solar, Inc. Abstract The trade-off between thick (~170 microns) silicon-based PV and thin (a few microns) film non-silicon and amorphous silicon PV is addressed
Silicon Drift Detector Product Brochure Update 2013 Content Classic Silicon Drift Detector High Resolution Silicon Drift Detector Multielement Silicon Detector Extra Large Detector Series July 2013 About
International Journal of Electronics and Computer Science Engineering 1482 Available Online at www.ijecse.org ISSN- 2277-1956 Behavioral Analysis of Different ALU Architectures G.V.V.S.R.Krishna Assistant
Application Note for SDP600 and SDP1000 Series Measuring Differential Pressure and Air Volume with Sensirion s CMOSens technology Summary The increasing customer requirements for comfort and safety and
Comparison study of FETs: SOI vs. Bulk Performance, Manufacturing Variability and Cost David Fried, IBM Thomas Hoffmann, IMEC Bich-Yen Nguyen, SOITEC Sri Samavedam, Freescale Horacio Mendez, SOI Industry
Lecture 22: Sequential Circuits Latches: SR D JK Flip-Flops Memory Sequential Circuits In sequential circuits, new state depends on not only the input, but also on the previous state. Devices like registers
CHAPTER 1 INTRODUCTION 1.1 Background The command over cloud computing infrastructure is increasing with the growing demands of IT infrastructure during the changed business scenario of the 21 st Century.